Ana Roda 1,2, Ana A. Matias 2 , Alexandre Paiva 1 and Ana Rita C. Duarte 1,*
1 LAQV, REQUIMTE, Departamento de Química da Faculdade de Ciências e Tecnologia, Universidade Nova de Lisboa, 2829-516 Caparica, Portugal; [email protected] (A.R.); [email protected] (A.P.) 2 iBET, Instituto de Biologia Experimental e Tecnológica, Apartado 12, 2781-901 Oeiras, Portugal; [email protected] * Correspondence: [email protected]; Tel.: +351-212-949-680
Received: 24 April 2019; Accepted: 17 May 2019; Published: 21 May 2019
Abstract: The green and versatile character of deep eutectic solvents (DES) has turned them into signiﬁcant tools in the development of green and sustainable technologies. For this purpose, their use in polymeric applications has been growing and expanding to new areas of development. The present review aims to summarize the progress in the ﬁeld of DES applied to polymer science and engineering. It comprises fundamentals studies involving DES and polymers, recent applications of DES in polymer synthesis, extraction and modiﬁcation, and the early developments on the formulation of DES–polymer products. The combination of DES and polymers is highly promising in the development of new and ‘greener’ materials. Still, there is plenty of room for future research in this ﬁeld.
Keywords: deep eutectic solvents; polymers; green chemistry; synthesis; extraction; formulation
1. Introduction Deep eutectic solvents were ﬁrst described by Abbot in 2002 , referring to the liquid formed just by mixing quaternary ammonium salts with metal salts, at ambient temperature. The term ‘eutectic’ was ﬁrst introduced at the end of the 19th century (1884). By deﬁnition, it refers to the minimum freezing/melting temperature achieved by a mixture of two or more compounds at a particular molar ratio . However, the deep eutectic solvents (DES) concept is often not restricted to a unique ratio of compounds, being commonly deﬁned as a mixture of two or more compounds with a lower freezing/melting point lower than the pure components. This concept opens a larger spectrum of DES options with tunable properties . The mechanism of DES formation is not yet well understood but it most probably occurs through hydrogen bonding, electrostatic interactions and/or Van der Waals interactions [4–8]. Since there is no consensual deﬁnition for DES in the scientiﬁc community, all the papers reporting the use of DES, under their own deﬁnition, were considered in this review. The exponential concern with environmental issues highly motivated the development of green technologies. DES have emerged as green solvents due to their low toxicity and volatility, biodegradability, biocompatibility, easy production, high yields and purity, and the fact that they are widely available precursors [9,10]. This type of solvent can fulﬁll the principles of green chemistry [11,12] while being highly tunable for several distinct areas. Good examples of DES that “fully represent green chemistry principles” are natural DES (NADES), a subclass of DES formed by compounds from natural origin [13–15]. Throughout the last decade, an exponential interest has been given to the research on DES, a rate expected to maintain if not to increase (Figure1a). Up until now, deep eutectic solvents
Polymers 2019, 11, 912; doi:10.3390/polym11050912 www.mdpi.com/journal/polymers Polymers 2019, 11, 912 2 of 22 Polymers 2019, 11, x FOR PEER REVIEW 2 of 24
Throughout the last decade, an exponential interest has been given to the research on DES, a rate have alreadyexpected been reportedto maintain if for not several to increase applications, (Figure 1a). Up primarilyuntil now, deep for eutectic electrochemistry, solvents have already synthesis and extraction [14been,16 , reported17]. for several applications, primarily for electrochemistry, synthesis and extraction [14,16,17]. Polymers 2019, 11, x FOR PEER REVIEW 2 of 24
Throughout the last decade, an exponential interest has been given to the research on DES, a rate expected to maintain if not to increase (Figure 1a). Up until now, deep eutectic solvents have already been reported for several applications, primarily for electrochemistry, synthesis and extraction [14,16,17].
Figure 1. NumberFigure 1. of Number published of published articles articles per per year year on on ((aa)) deep eutectic eutectic solvents solvents and (b and) deep ( beutectic) deep eutectic solvents and polymers. Data from Web of Knowledge . solvents and polymers. Data from Web of Knowledge . (a) (b) Within all the reported studies, ~8% correspond to the use of DES in polymeric applications . Figure 1. Number of published articles per year on (a) deep eutectic solvents and (b) deep eutectic The investigation on this field largely increased in the recent years (Figure 1b), including Within all thesolvents reported and polymers. studies, Data ~8% from Web correspond of Knowledge  to.the use of DES in polymeric applications . The investigationsolubilization, on this extraction, ﬁeld largely synthesis increased, or modification in the recentof polymers. years The (Figure most recent1b), studies including report solubilization, DES incorporationWithin in all the the f reportedormulation studies, of polymeric ~8% correspond products. to the The use currentof DES in relative polymeric incidence applications of the  different. extraction, synthesis, or modiﬁcation of polymers. The most recent studies report DES incorporation areasThe herein investigation explored onis represented this field largely in Figure increased 2. in the recent years (Figure 1b), including in the formulationsolubilization, of polymeric extraction, products. synthesis, or modification The current of polymers. relative The incidence most recent studies of the report diﬀ DESerent areas herein explored is representedincorporation in in Figurethe formulation2. of polymeric products. The current relative incidence of the different areas herein explored is represented in Figure 2.
Figure 2. Graphical representation of the relative incidence of the subareas explored within deep eutectic solvents (DES)–polymer field . Figure 2. GraphicalFigure 2. representation Graphical representation of the of the relative relative incidence incidence of the of subareas the subareas explored within explored deep within deep eutectic solvents (DES)–polymer field . eutectic solventsStill, it (DES)–polymer seems that the DES ﬁeld versatility . regarding polymers seems to be broadening. This review summarizesStill, it the seems explored that the DES applications versatility regarding of DES andpolymers polymers, seems to ai beming broadening. to consolidate This review current Still, it seemsachievementssummarizes that theand the to DES explored promote versatility applications further developments. regarding of DES andpolymers polymers, ai seemsming to to consolidate be broadening. current This review summarizes theachievements explored applicationsand to promote further of DES developments. and polymers, aiming to consolidate current achievements 2. Fundamental Studies Involving DES and Polymers and to promote2. further Fundamental developments. Studies Involving DES and Polymers The investigation of deep eutectic solvents for several applications has been growing at a fast The investigation of deep eutectic solvents for several applications has been growing at a fast pace. The fundamental knowledge of their properties for those applications is hence crucial for their 2. Fundamentalpace. Studies The fundamental Involving knowledge DES of and their properties Polymers for those applications is hence crucial for their optimizationoptimization and and development. development. Although Although DES DES are are frequently frequently fully fully characterized characterized as individual as individual The investigationsystems,systems, the the intra of intra deep- and- and inter eutecticinter-interactions-interactions solvents inin thethe forapplication application several context context applications are areessential. essential. The has fundaThe been fundamental growingmental at a fast pace. The fundamentalstudiesstudies involving involving knowledge DES DES and and polymers polymers of their are properties scarcescarce, ,as as expected expected for thoseof ofnovel novel applicationsapplications, applications, hence ishence we hence present we present crucial for their herehere studies studies reported reported within within this this topictopic in thethe last last 3 3years. years. optimization and development. Although DES are frequently fully characterized as individual systems, In 2016, Sapir et al. studied the molecular solvation of poly(vinyl pyrrolidone) (PVP) polymer in the intra- and inter-interactionsIn 2016, Sapir et al. studied in the the applicationmolecular solvation context of poly(vinyl are essential. pyrrolidone) The (PVP) fundamental polymer in studies cholinecholine chloride:urea chloride:urea 1:2 1:2 (molar (molar ratio) ratio) DES, inin comparison comparison to towater, water, through through conformational conformational and and involving DES and polymers are scarce, as expected of novel applications, hence we present here studies reported within this topic in the last 3 years. In 2016, Sapir et al. studied the molecular solvation of poly(vinyl pyrrolidone) (PVP) polymer in choline chloride:urea 1:2 (molar ratio) DES, in comparison to water, through conformational and thermodynamic analysis. Despite the similarity of DES and water as solvents for PVP, the authors reported diﬀerent intermolecular interactions between PVP-DES and PVP–water. According to Flory Huggins Solution Theory, the PVP individual interactions are more similar to the DES’ than − water interactions, favoring PVP-DES interaction. Their results supported this DES as a “close-to-ideal” solvent for PVP . Similar studies were carried out for poly(ethylene oxide) (PEO) polymer in 1:2 (molar ratio) DES of ethylammonium bromide (EABr):glycerol, EABr:ethylene glycol, or butylammonium bromide (BABr):glycerol. The results characterize the tested DES as moderately good Polymers 2019, 11, 912 3 of 22 solvents for PEO with higher quality for ethylene glycol than glycerol-based DES . Moreover, they postulate that the higher density of hydrogen bonds per unit volume and the availability of such interactions improves the DES solvation capacity. Fundamental data on the inﬂuence of the DES hydrogen networking in its 3D structure can be acquired to predict its solvation capacity and used as a preselection parameter for certain applications. An example is the work of Hammond et al. on neutron diﬀraction and atomistic modelling to acquire the probable liquid structure of choline chloride–urea DES . Considering DES–polymer systems, this type of preliminary information for several DES systems and/or diﬀerent component ratios could be used to select or adjust suitable DES for polymer solvation. However, the DES–polymer systems are more complex than DES in its isolated form. It is then necessary to study the combined system to have more accurate information on their interaction. In this context, Stefanovic and his coworkers performed a systematic quantum chemical investigation on the PEO solvation in DES of choline chloride (ChCl) mixed with urea, ethylene glycol, or glycerol. The solvation conformation of PEO was correlated with the type of hydrogen bond donor, the density of hydrogen bonds in DES and the inﬂuence of PEO in the hydrogen network. ChCl:urea had the strongest and denser hydrogen network, whereas ChCl:glycerol presented the weakest and less dense. Interestingly, the PEO ChCl:urea disrupted the weaker hydrogen bonds, strengthening the robust ones, which caused a highly structured solvation environment, ‘imprisoning’ the PEO in a static and coiled conformation. On the contrary, in the least structured environment of ChCl:glycerol, the polymer presented a free conformational structure . A diﬀerent study, conducted by Hillman et al. observed the intrinsic composition of DES and the extrinsic coupled conditions needed for electrochemical deposition of polyaniline (PANI) in aqueous media and DES of ethylene glycol:choline chloride or oxalic acid:choline chloride. Furthermore, the inﬂuence of DES as electrolytes in the electroactivity of the produced PANI-based ﬁlms was studied and evaluated in terms of ﬁlm longevity and charge storage stability after successive redox cycles. The oxalic acid-based DES electrolyte was better for PANI electrodeposition, with no further additives, whereas ethylene glycol-based DES required the addition of sulfuric acid as a protic source . Thermodynamic investigation of phase equilibrium involving DES:polymer:water systems was carried out by Baghlani and Sadeghi. DES of choline chloride with urea, ethylene glycol or glycerol 1:2 molar ratio and the water-soluble polymers polypropylene glycol400 (PPG400), polyethylene glycol400 (PEG400), and polyethylene glycol10000 (PEG10000) were used to prepare diﬀerent DES/polymer/water ternary systems. Their water activity was determined through the isopiestic method. The authors observed that the DES:PPG:H2O mixture formed two immiscible aqueous phases, called aqueous biphasic systems (ABS), due to the incompatibility of both polymer and DES to form hydration complexes. Speciﬁcally, the choline chloride and glycerol caused soluting-out of the polymer. This mechanism was depended on the competition between hydrogen bonding and hydration. Similar studies on ABS have been reported by Freire et al. for ionic liquids, also contemplating polymer-based ABS .
3. Polymeric Synthesis Using DES The ﬁrst article identiﬁed reporting polymerization using an eutectic mixture was published in 1985 , 100 years after Guthrie published the eutectic deﬁnition . In that study, Genies and Tsintavis compared the preparation of the polyaniline polymer by electrochemical polymerization in a eutectic mixture of NH4F-HF to other media (aqueous and organic). By that time, they could already identify the eutectic solvent as an advantage over the use of other solvents. The polyaniline polymers produced in the eutectic mixture presented better nucleation and polymerization process, with almost 100% yield, as opposed to other media. Additionally, it was also better in terms of adherence and electrochemical properties for all the preparation conditions studied. Over the years, other studies were conducted on the synthesis of natural and synthetic polymers evolving eutectic mixtures [26–28], but only in 2011 the term ‘deep eutectic solvent’ was used by Mota-Morales et al. for polymerization studies . Polymers 2019, 11, 912 4 of 22
3.1. DES as Functional Monomers In the study of Mota-Morales et al., the authors used mixtures of choline chloride with acrylic acid or methacrylic acid monomers to form DES, providing both media and functional monomer for frontal polymerization. From their knowledge in similar works using ionic liquids, they could tailor the ratio of DES components to enhance polymer conversion through a suitable content of double bonds and by stabilizing the reaction temperature and velocity through the high viscosities of the prepared DES. Moreover, once the monomer units contained in the DES were polymerized, it was possible to reutilize the choline chloride component. The mentioned process allowed the utilization of the DES as a medium and functional monomer for polymerization while demonstrating an enhanced performance in comparison to conventional organic solvents and ionic liquids . DES enhanced the polymerization process at four diﬀerent levels: (i) through the reduction of components for reaction, (ii) by acting as an alternative solution to organic solvents with improved performance, (iii) minimization of the waste produced, and (iv) recycling of the remnant compounds. These features highly enrich the “green” value of DES. Additional studies about the use of DES as a functional monomer for polymerization were published. The groups of Xu, Wang J. and Wang R. reported the polymerization of choline chloride:itaconic acid (ChCl:IA), using IA as a monomer unit, for the preparation of solid extraction matrices [30,31] or stationary phase for chromatographic separation . Xu et al. noticed unique benefits of DES polymer incorporation in the extraction system in terms of its stability, surface area, and moldable structure . In turn, Wang J. et al., mentioned the potential of different monomer compositions in DES to produce tuned-sorbents for extraction . In another work, Isik et al. produced poly(ionic liquids) for CO2 sorption by photopolymerization of DES monomer units formed by 2-cholinium methacrylate bromide monomer and natural carboxylic acids, amidoximes, or amine . A more recent paper described a novel DES of 3-acrylamidopropyl trimethylammonium chloride (APTMACl):d-sorbitol 2:1 (molar ratio) as a monomer for polymerization on the surface of amino magnetic metal–organic framework ([email protected]). This DES was designed for the functionalization of [email protected], not only through polymerization but also by coordination of DES-nitrogen and HKUST-1. The functionalization with DES incorporated hydrogen and ionic interactions on the surface of the MOF sorbent, which improved its function in the extraction of cationic dyes .
3.2. Electrochemical Polymerization Electropolymerization was also mentioned in Mota-Morales and coworkers’ review. It consists in the polymerization of monomers through electrochemical induction that leads to the formation of conductive polymers, normally in the form of electrodeposited ﬁlms . An interesting feature of using DES as media for electropolymerization is its inﬂuence in the polymer formation and its ﬁnal characteristics [36,37]. This type of polymerization is one of the ﬁrst applications of DES, reported in the 1980s, as stated by Fernandes et al. in their article about polyaniline (PANI) electrosynthesis in DES. PANI electropolymerization rates in DES of choline chloride with ethylene glycol, urea or glycerol showed to be determined by the viscosity and conductivity of those solvents . Using the same DES systems, Prathish et al. published the electropolymerization of poly(3,4-ethylenedioxythiophene) (PEDOT), with better results of stability and sensitivity for the PEDOT prepared from choline chloride:urea DES. The shape, size, surface, electrocatalytic, and sensing properties of the PEDOT ﬁlms were highly inﬂuenced by the DES used [37,39]. The most recent study reported on this topic, from Zou and Huang, also focused the electrodeposition of PANI from DES. The novelty of their work is the electropolymerization without exogenous acid as a proton source, by using newly synthesized DES, of proton-functionalized anilinium hydrochloride ([HANI]Cl) or anilinium nitrate ([HANI]NO3) with glycol. The authors tailored the ratio of anilinium salt:glycol in terms of conductivity and obtained a ﬁnal DES with high conductivity and low viscosity, highly suitable for electropolymerization . Table1 resumes the polymers synthesized through electropolymerization, the DES used for that purpose, their function, and the potential applications of the produced products. Polymers 2019, 11, 912 5 of 22
Table 1. Summary of DES and their function in electropolymerization, polymers produced, and their potential applications.
DES (molar ratio) Function Polymer synthesized Application Ref. ChCl:ethylene glycol 1:2 Solvent Electrochromic devices, ChCl:urea 1:2 Polyaniline  Electro-modiﬁer supercapacitors ChCl:glycerol 1:2 ChCl:ethylene glycol 1:2 Solvent Poly(3,4-ethylenedioxythiophene) ChCl:urea 1:2 Sensing of biomarkers [37,39] Inﬂuence in PEDOT properties (PEDOT) ChCl:glycerol 1:2 Electrochemical sensors ChCl:ethylene glycol 1:2 Solvent Poly(methylene blue) [41,42] biomarkers Proton-functionalized anilinium hydrochloride ([HANI]Cl) or anilinium Solvent Polyaniline Capacitors  nitrate ([HANI]NO3) with glycol 1:10 Polymers 2019, 11, 912 6 of 22
3.3. Polycondensation Polycondensation occurs in polymer synthesis by condensation reactions through molecular combination with liberation of small molecules (byproduct), normally forming polymeric matrices . This type of polymer synthesis is commonly used for the production of carbon-based materials. The review of Carriazo et al. from 2012, refer some polycondensation studies with DES , however the investigation on this topic is still scarce. In the last 5 years, three representative studies of polycondensation in DES were published [45–47]. Lopéz-Salas et al. reported resorcinol:urea (3.5:1 molar) and resorcinol:urea:choline chloride (3.5:0.5:1, 3.5:1:1, and 3.5:2:1 molar, respectively) DES for tailoring the structure of hierarchical porous carbons. In their study, the urea content in DES allowed controlling the pore dimensions of the produced matrices . Patiño et al. used DES of resorcinol:3-hydroxypyridine (1:2:1 molar) or resorcinol:tetraethylammonium bromide (1:3:1.75 molar) as polycondensation solvent to produce hierarchical nitrogen-doped carbon molecular sieves . Chen et al. published the use of 1:2 (molar ratio) choline chloride:urea DES as a solvent for the two-stage polymerization from phenol and formaldehyde, to produce porous carbon xerogels . Interestingly, in both Chen and Patiño works, DES act as a homogenization medium, structure-directing agent and as a nitrogen source for carbons [45,46].
3.4. Molecular Imprinted Polymers with DES Molecular imprinted polymers (MIPs) are molds made by polymerization around template molecules, for its speciﬁc recognition. By molding speciﬁc structures and size in the polymeric matrix, the MIPs are able to speciﬁcally recognize and hold the molded template by complementary match [48,49]. These polymer molds are used for recognition and separation, puriﬁcation, production of artiﬁcial antibodies, target delivery and/or electrochemical sensors . One of the most recent applications of DES is its use for the production of MIPs, either as medium or solvent [50,51], as MIPs modiﬁer [51–63], as MIPs functional monomer [48,53,54,64–72], and even as MIPs template [67,69] (Table2). From the whole publications involving DES and polymers, more than 15% correspond to DES and MIPs, reported just in the last four years . In 2016, Li et al. described for the ﬁrst time the use of DES for the modiﬁcation of MIP. The authors postulated that the interaction of DES with the functional monomer, and/or the surface of MIP, improved aﬃnity, selectivity and adsorption of chlorogenic acid . In the same year, Liu et al. reported the use of DES as a functional monomer for MIPs polymerization: DES-MIP. The produced DES-MIPs have shown to be stable, reusable, have a high imprinting factor, fast binding kinetics, and high adsorption capacity. The authors described the produced DES-MIPs as ‘outstanding’ for the speciﬁc and selective recognition of bovine hemoglobin from protein mixtures or real samples . All the following works showed similar features, supporting DES-MIPs as highly eﬃcient and selective in the recognition of the template molecules. Some authors also reported the advantages of the produced DES-MIPs in comparison with MIPs from conventional monomers [52,53,56,66]. According to Li G. et al., Li X. et al. (2017), and Xu et al., DES have an advantage over conventional monomers due to their high content in available functional groups, allowing unique interactions with the template molecules, which translates into higher aﬃnity and selectivity for the respective DES-MIPs [48,52–54,57,62]. Li G. and its coworkers also postulated that increasing DES-MIPs rigidity can prevent its shrinkage or swelling [53–56]. Moreover, the liquid character of DES may also be an advantage by including the monomer in the bulk of DES or by substituting the need of media or solvent when used as an additive. The most recent paper reported on DES-MIPs showed some innovative features. Fu and coworkers prepared DES-MIPs in a 2D material as a surface, using a 1:2 molar ratio mixture of choline chloride and acrylic acid DES, as functional monomer. The use of this technique avoids the immersion of the template during polymerization, facilitating its removal. The produced polymeric matrix presented the required biomolecule recognition and showed to be renewable. Additionally, it presented antibacterial activity, a high added value feature for analyzing or delivering additives to biosamples while preserving them . Polymers 2019, 11, 912 7 of 22
Table 2. Summary of the work reported in the literature regarding DES-molecular imprinted polymers (MIPs).
DES (molar ratio) Function Application Description Ref. MIPs modiﬁer: interaction with Selective recognition and separation DES-MIPs are more rigid, preventing shrinking or swelling; ChCl:glycerol 1:2  a functional monomer of chlorogenic acid from honeysuckle DES-MIP showed higher adsorption capacity than MIP DES-MIPs showed a much higher adsorption capacity, rapid binding kinetics, and high imprinting factor for the BHb, Functional monomer Selective recognition and separation compared with the magnetic DES-NIPs (NIP = ChCl:methacrylic acid 1:2  for polymerization of bovine hemoglobin (BHb) protein nonimprinted polymers); Magnetic DES-MIPs presented highly recognition, speciﬁcity and selectivity ChCl:ethylene glycol 1:3 Selective recognition and extraction MIPs modiﬁer: interaction with DES-MIPs of ChCl:glycerol 1:3 showed the best results, in ChCl:glycerol 1:3, 1:2, 1:4, 1:6 of rutin, scoparone, and quercetin  a functional monomer comparison to other DES and MIPs ChCl:1,4-butanediol 1:3 from Herba Artemisiae Scopariae The polymeric resins prepared in DES had higher adsorption Recognition of clorprenaline and ChCl:ethylene glycol 1:2 Solvent capacity than the ones prepared in alcoholic solvents;  bambuterol in urine 100% DES used as a polymerization solvent MIPs modiﬁer: interaction with Puriﬁcation of chloromycetin and Higher extraction recoveries for DES-MIPs, than for MIPs ChCl:glycerol 1:2  a functional monomer thiamphenicol from milk and NIPs ChCl:ethylene glycol 1:1 Adsorption capacity of DES-MIPs better than MIPs; MIPs modiﬁer: interaction with ChCl:glycerol 1:1 Screening chloramphenicol in milk ChCl:EG-based DES-MIPs had the best adsorption ability and  a functional monomer ChCl:propylene glycol 1:1 higher recoveries than MIPs and C18 Adsorption of levoﬂaxacin or MIPs modiﬁer: interaction with The DES-MIPs showed better eﬃciency in recognition and Betain:ethylene glycol:water 1:2:1 tetracycline from a millet extraction  a functional monomer speciﬁc adsorption than MIPs with a mixture of other antibiotics DES-MIPs showed better adsorption capacity and higher MIPs modiﬁer: interaction with Recovery of levoﬂoxacin from green Betaine:ethylene glycol:water 1:2:1 recoveries of levoﬂoxacin than MIPs, NIPs, Mesoporous  a copolymer bean extract, through SPE Siliceous Material (MSM), DES-MSM, and C18 ChCl:ethylene glycol 1:2 ChCl:glycerol 1:2 ChCl:1,4-butanediol 1:2 Puriﬁcation of alkaloid isomers MIPs modiﬁer: interaction with DES-MIPs of ChCl-urea 1:2 showed the best results, in ChCl:formic acid 1:2 (theobromine and theophylline) from  a functional monomer comparison to other DES and ionic liquid modiﬁed-MIPs ChCl:acetic acid 1:2 green tea ChCl:propionic acid 1:2 ChCl:urea 1:2 Polymers 2019, 11, 912 8 of 22
Table 2. Cont.
DES (molar ratio) Function Application Description Ref. Formic acid: methylltriphenylphosphonium Functional monomer and Selective recognition of rutin and bromide: chalcone 1:0.5:0.05-based DES-MIP had the best adsorption capacity  dummy template quercetin from molecular mixtures (FA:Mtpp:Chal) 1:0.5:0.04, 1:0.5:0.05, 1:0.5:0.06, Caﬀeic acid: ChCl:Formic acid Functional monomer Adsorption of levoﬂoxacin from DES-MIPs of 1:3:1.5 CA:ChCl:FA more selective for detection (CA:ChCl:FA)  for polymerization millet extract and puriﬁcation of levoﬂoxacin 1:3:1.5, 1:4:2, 1:6:3 ChCl:ethylene glycol 1:3 ChCl:glycerol 1:3 ChCl:1,4-butanediol 1:3 Recognition of fucoidan and alginic Best recovery using the ChCl:urea based DESs-magnetic MIPs ChCl:urea 1:3 MIPs modiﬁer acid from seaweed by magnetic The best DESs-magnetic MIPs was better than the respective  ChCl:formic acid 1:3 solid-phase extraction MIPs and NIPs ChCl:acetic acid 1:3 ChCl:propionic acid 1:2 1:0.4:1-based DES-MIPs had the best adsorption capacity; DES-MIPs had better speciﬁc recognition and larger ChCl: caﬀeic acid:ethylene glycol 1:0.1:1, Template and Recognition of polyphenols adsorption abilities than NIP, C18, and C8;  1:0.2: 1, 1: 0.3:1, 1:0.4:1 functional monomer Recognition of CA from polyphenol mixtures and in a real sample ChCl:ethylene glycol 1:2 ChCl:glycerol 1:2 Best recovery for the ChCl:urea-based ChCl:1,4-butanediol 1:2 Puriﬁcation of D-(+)-galactose, [email protected]; ChCl:urea 1:2 MIPs modiﬁer L-( )-fucose, and D-(+)-mannose  − The best [email protected] system was better than the ChCl:formic acid 1:2 from seaweed, though SPE respective [email protected], DES-HMIPs, and DES-NIPs ChCl:acetic acid 1:2 ChCl:propionic acid 1:2 DES-MIPs showed a good adsorption capacity, with a higher Allyltriethylammonium Functional monomer imprinting factor and higher speciﬁcity than other MIPs for Adsorption of lysozyme  Chloride ([ATEAm]Cl):glycerol 1:1 for polymerization lysozyme puriﬁcation; 4 times recyclable Extraction of tanshinone I, IIA, and cryptotanshinone from Salvia Multiple template DES-MIPs reduced the experimental steps; ChCl:urea 1:2 miltiorrhiza bunge; glycitein, genistein, The DES-MIPs tested were better than NIPs and MIPs, except ChCl:ethylene glycol 1:2 MIPs modiﬁer and daidzein from Glycine max (Linn.) for the ChCl-urea-based DES-MIP;  ChCl:1,4-butanediol 1:2 Merr; and epicatechin, Best extraction recoveries for ChCl-glycerol-based DES-MIP; ChCl:glycerol 1:2 epigallocatechin gallate, and DES-MIPs can be reused epicatechin gallate from green tea Polymers 2019, 11, 912 9 of 22
Table 2. Cont.
DES (molar ratio) Function Application Description Ref. Separation of (+)-catechin, ChCl:methacrylic acid (MAA) 1:2 ( )-epicatechin, and Higher recoveries with DES-MIPs than MAA-MIPs or NIPs; Functional monomer −  Betaine/MAA/H O 1:2:1 ( )-epigallocatechin gallate from The ChCl-MAA bases DES-MIP had slightly better results 2 − black tea ChCl:oxalic acid:ethylene glycol 1:1:1, Selective recognition and separation 1:1:2, 1:1:3 The ChCl:OA:PG based DES-MIPs has the best recovery of theophylline, theobromine, ChCl:oxalic acid:glycerol 1:1:3 Functional monomer results and was better than the respective DES-NIP, MIP, NIP,  (+)-catechin hydrate, and caﬀeic acid ChCl:oxalic acid:propylene glycol 1:1:1 and MIPs made from conventional monomers (MAA and AM) from green tea ChCl:caﬀeic acid:ethylene glycol 1:1:1 Isolation of transferrin from ChCl:acrylic acid 1:2 Additive functional monomer Selective adsorption over protein mixtures  human serum DES used for modiﬁcation of MIPs by interaction with the ChCl:formic acid 1:2 functional monomer; ChCl:acetic acid 1:2 MIPs modiﬁer: interaction with Selective recognition and separation DES-MIPs of ChCl-urea 1:2 showed the best results, in  ChCl:propionic acid 1:2 a functional monomer of Fucoidan and Laminarin comparison to other DES, ionic liquid modiﬁed-MIPs and ChCl:urea 1:2 nonmodiﬁed MIPs DES-MIPs showed higher recoveries than MIPs, NIPs, and the corresponding DES-NIPs; Template and Extraction of 3,4-dihydroxybenzoic 1:1:2 ChCl:DHBA:EG-based DES-MIPs showed the highest ChCl:DHBA:EG 1:1:1, 1:1:2, 1:1:3  functional monomer acid (DHBA) recoveries of 3,4-DHBA and better adsorption capacity, imprinted factor, and selectivity than the conventional functional monomer 4-vinylpyridine Functional monomer Separation of bovine hemoglobin DES-MIPs separated eﬀectively BHb from calf blood; (APTMACl):urea 1:2  for polymerization from a complex sample DES-MIPs could be recycled at least 3 times The binary green system was the unique solvent used for all Binary green solvent and MIP the polymerization reagents; ChCl:ethylene glycol 1:2, 1:3, 1:4 modiﬁer: porogen (mixture Drug delivery of Fenbufen  It was also a good dispersant for the single-walled with ionic liquid) carbon nanotubes DES-MIPs better than DES-NIPs; Determination of Levoﬂoxacin in ChCl:ethylene glycol 1:2 MIPs modiﬁer: porogen DES-MIPs eﬃciently applied to examine levoﬂoxacin from  human plasma human plasma of hospitalized patients Surface DES-MIPs prepared to facilitate further template removal; Recognition and good antibacterial ChCl:acrylic acid 1:2 Functional monomer The produced polymeric system presented good adsorption  properties for β-lactoglobulin in milk and selectivity for β-lactoglobulin, was reusable, and showed antibacterial activity Polymers 2019, 11, 912 10 of 22
3.5. Other Types of Polymer Synthesis Free radical polymerization is one of the most common types of polymerization. Mota-Morales et al. (2017) published a very complete review of polymerization using DES focusing on the ‘free radical polymerization’ of and in ‘deep eutectic solvents’. Herein, we make a brief summary of the main outcomes mentioned in their work and recommend the consultation of their review as a complement to this section. It states the high plasticity of DES, either in terms of composition, molar ratios and the broad range of interactions. The authors describe the use of DES as inert solvent and/or reactive component, focusing the ‘all-in-one’ systems when both functions are combined. They summarize the polymerizable DES, the polymer resulted from their free radical polymerization and their application. Their review highlights the green character of DES, its ‘greening’ impact in the polymerization process and in the product formed. In addition, it presented the potential of DES as a broadener of the synthetic conditions (e.g., temperature and vacuum) in comparison to other solvents, creating new polymerization strategies . After this comprehensive review, innovative work has been developed in the ﬁeld. Ferreira et al. synthesized chondroitin sulfate mesoporous materials by using DES for biopolymer dissolution and mesoporous templating. Despite the lack of knowledge about the exact templating mechanism, the authors suggested that DES can act as a capping agent and/or as ﬁller. Mesoporosity was eﬀectively obtained by including DES in this biopolymer composite synthesis, while a stable structure was maintained after DES removal . In turn, Maximiano and coworkers published the ﬁrst article reporting the use of DES as cosolvent in ethanol for supplemental activator and reducing agent atom transfer radical polymerization (SARA ATPR) . Following this new development, Wang et al. and Mendonça et al. published the ﬁrst studies on the use of diﬀerent DES as ligand , as 100% solvent for SARA ATPR  or both . Other studies also reported the use of DES as solvent medium for polymer synthesis [46,79–90]. In particular, the communication of Park and Lee on the polymerization of 3-octylthiophene in DES presented interesting features regarding the use of DES as a solvent in polymerization. DES of choline chloride:urea improved polymerization yield and duration in comparison to chloroform and the best ionic liquids for that purpose. The hydrogen bond basicity of the DES used showed to be preeminent for the eﬀective polymerization of that polymer . Furthermore, a more recent work published the use of ChCl:glycerol 1:2 molar ratio DES as reaction media for oleoﬁn anionic polymerization . The authors highlighted the advantages of the protic and polar character of DES for the polymerization and reported that the selective use of glycerol as hydrogen bond donor instead of urea, lactic acid, or oxalic acid increased the polymerization performance. These examples emphasize, once again, the potential of DES versatility to be tailored for speciﬁc applications. The substitution of organic or other toxic solvents by green DES and its role in additional functions, simultaneously to solvent, is a great development in green chemistry.
4. Extraction of Polymers with DES Within the DES applications already reported, its use for the extraction of polymers has been widely explored. A recent review of Zdanowickz et al. (2018) reviewed the work developed regarding DES for extraction of polysaccharides, namely, lignin, cellulose, starch, agar, agarose, chitin, chitosan, xylan, pectin, and inulin. It summarizes the DES used for the extraction of these polymers from diﬀerent biomasses, either for separation from the raw materials or for polysaccharides recovery/puriﬁcation, through solubilization or induction of ﬁbrillation or crystallization. It also addresses the use of DES for obtaining low molecular products from polymers degradation or sacchariﬁcation . Moreover, several reviews address polymer extraction with DES from lignocellulosic biomass, one of the most explored raw materials regarding processing with DES [91–93]. As a result of the intense investigation on the topic, the discoveries are steadily uncovered. In the present review, recently published works involving DES in polymer extraction are listed in Table3, summarizing the DES composition, the polymers extracted, the raw material used for extraction and Polymers 2019, 11, 912 11 of 22 some additional information about the cited papers. Some previously reported studies on this topic are available in the review of Zdanowickz et al. . In a paper of Saravana et al., they tested 14 diﬀerent DES for chitin extraction from shrimp waste. All the DES presented higher yields than the conventional extraction method and ChCl:malonic acid was the more selective DES for pure chitin. Additionally, ﬁlms from the extracted chitin were eﬃciently produced, with similar characteristics to ﬁlms from commercial chitin . In terms of the parameters inﬂuencing polymer extraction using DES, Bai et al., and Mammilla et al. reported the DES acidity, viscosity, and the content in free hydrogen proton as main features inﬂuencing their extraction eﬃciency [95,96]. Moreover, the solubility of the target polymer in the DES is obviously crucial for the extraction eﬃciency. The reviews of Melro et al. and Duan et al. summarized DES found to be suitable for the dissolution of lignin  and chitin , the most commonly extracted polymers with DES. Additional features regarding the DES mechanisms for extracting polymers are normally not referred, probably by assuming to be basic extraction principals. Herein, we present some of those basic concepts, focusing polymer extraction with DES and infer some unique possible contributions of the DES for this application. The diﬀusion of DES into the matrix containing the extractable polymer and the mass transfer interactions of DES–matrix–polymer are decisive factors. The ionic content and hydrogen bonding capacity of DES is highly promising for mass transfer improvement and for rupturing conformational chemical bonds of the matrix, facilitating solvent diﬀusion. Furthermore, as referred in the previous sections for other applications, DES can establish hydrogen and electrostatic interactions with the functional groups of a target molecule, conferring them higher aﬃnity to each other. This principle is applicable to polymers extraction with DES. The knowledge of the molecular structures involved in the extraction and their possible interactions can be used to tailor the extraction yield and/or extraction selectivity of target polymer(s).
Table 3. Summary of some reported studies on polymer extraction with DES, from 2017 to 2019.
DES (molar ratio) Polymer extracted Raw material Description Ref. ChCl:urea (U) 1:2 Extraction abilities: ChCl:OA > ChCl:HAc ChCl:ethylene glycol (EG) 1:2 > ChCl:La > ChCl:EG > ChCl:GOH ChCl:glycerol (GOH) 1:2 > ChCl:U; ChCl:lactic acid (LA) 1:2 Collagen Cod skin Better extraction eﬃciency for 1:1  ChCl:acetic acid (HAc) 1:2 ChCl:oxalic acid; ChCl:oxalic acid (OA) 1:1, Extraction inﬂuenced by the DES viscosity, 1:0.8, 1:0.6, 1:1.2 acidity, and free hydrogen protons 1:2 of ChCl with lactic acid, Highest yield obtained for the DES of 1,4-butanediol, ethylene ChCl:oxalic acid, but the most selective glycol, urea, 1,6-hexanediol, Shrimp shells (purest chitin) was ChCl:malonic acid DES; glycerol, oxalic acid, malonic Chitin (Marsupenaeus Higher yields than conventional extraction  acid, citric acid, malic acid, japonicas) for all DES tested; propylene glycol, Extracted chitin formed ﬁlms with similar L-(+)-tartaric acid, maleic properties to ﬁlms from commercial chitin anhydride, or thiourea Extraction assisted with dialysis ChCl:oxalic acid 1:2 Keratin Wool  High solubility of wool in the DES Eﬃcient dissolution and extraction of ChCl:oxalic acid 1:2 Keratin Rabbit Hair keratin from rabbit hair;  Extraction assisted with dialysis Eﬃcient extraction of chitin, ChCl:malic acid 1:1 Chitin Shrimp shells  demineralized and deproteinized ChCl:lactic acid (LA) 1:2 Oxalic acid and urea-based DES (acidic) ChCl:urea (UA) 1:2 Wood sawdust Lignin and were selective for lignin extraction, while ChCl:oxalic acid (OA) 1:1, 1:2 of beech  cellulose ChCl:KOH (alkaline) was selective for ChCl:potassium (Fagus sylvatica) extracting cellulose hydroxide 1:4 ChCl:lactic acid 1:9 Lignin Wood Lignin 80% pure  Polymers 2019, 11, 912 12 of 22
5. DES as Polymer Modiﬁcation Agents In the previous sections, the use of DES was mentioned as a modiﬁer agent, for example, in the synthesis of DES-MIPs as porogen or by incorporation of DES properties into the MIPs, conferring unique interactions to recognize target compounds. These unique interactions can occur through derivatization of the polymeric structures, either by derivatizing their own functional groups or by incorporating DES in the structure.
5.1. Derivatization Several studies were conducted on the use of DES as a derivatization agent by its inclusion in a polymeric material. We present here some examples. Wang and the coworkers reported the incorporation of DES into a polymer monolithic cartridge (DES-M), which could improve the aﬃnity and selectivity of the solid-phase extraction of quercetin from Ginkgo biloba. The observed advantages were attributed to the strong hydrogen bond network of the DES as a source of electrostatic and ionic interactions introduced in the surface of the DES-M during polymerization . Gan et al. also introduced DES (ChCl:glycerol 1:2 molar) as a modiﬁer in the polymeric synthesis of anionic-exchange resins, and as porogen and derivatization agent by its inclusion into the resin . Moreover, Li and Row incorporated aqueous DES of betaine mixed with glycerol, glucose, ethylene glycol or urea into mesoporous materials, improving their eﬃciency for dextrans separation . Other types of polymer derivatization using DES were published. Bangde et al. used ChCl:urea and ChCl:glycerol (1:2 molar) as chitosan methylation solvent. The urea-based DES was selective for N-methylation while glycine–DES systems also produced O-methylated chitosan. Both systems mediated eﬀectively chitosan methylation and presented advantages over the conventional method: (i) reduced organic solvent, (ii) decreased reaction time, and (iii) no polymer scission . A similar but innovative study reported O-acylation of chitin, directly converted from shrimp shells by DES. The wide versatility of these solvents, allowed for their simultaneous use for demineralization, deproteinization, and acylation initiator, while preventing the use of acids, bases, catalysts, and other acylating agents needed for the conventional method. Choline chloride:DL-malic acid 1:2 (molar ratio) were considered optimal for this purpose, within other ChCl:malic acid and ChCl:lactic acid DES systems . Cationic derivatization of polymers using DES has also been described [108,109]. Vuoti et al. used a boric acid:glycidyl trimethylammonium chloride 1:3 (molar ratio) DES mixture for the enhanced cationization of cellulose biopolymer, aimed wastewater treatment. The cationic cellulose derivatized by DES was eﬀectively used for water treatment, being a potential competitor to commercial polyacrylamides .
5.2. Plasticization DES have also been used as plasticizer of polymers. The review of Wong et al. comprises some general characteristics of plasticizers and their inﬂuence in polymers properties , listed in Table4.
Table 4. General characteristics of plasticizers and their inﬂuence in polymers properties.
Plasticizers characteristics Inﬂuence of plasticizers in polymers Decrease the melting or glass transition temperature Inert • • (Tg) of polymers Low molecular weight Preservation of the polymer elasticity • • Low vapor pressure Higher thermostability • •
According to these principals, deep eutectic solvents have suitable properties to be used as a plasticizer. Table5 compiles some DES used for the discussed purpose, the plasticized polymers, and the properties conferred. Those properties can change for diﬀerent polymers [111,112], and even for the same polymer with variations in structure or MW . In sum, the inﬂuence of DES in polymer Polymers 2019, 11, 912 13 of 22 plasticization depends on several factors, including DES composition, polymer type, DES:polymer ratio  and, of course, their speciﬁc interactions. An additional interesting feature also reported by Wong et al. is the possibility to use internal or external plasticizers, where the internal type usually implies the introduction of monomers into the polymeric matrix . Within the studies of DES as a plasticizing agent, we could not ﬁnd DES as a monomer for polymer plasticization. Since the use of DES as a functional monomer was already reported for the synthesis of polymeric structures, we would like to highlight its potential to be explored as monomer plasticizer. Still, within the context of the use of DES for polymer plasticization, Abbott et al. studied DES of ChCl:glycerol, ChCl:ethylene glycol, and ChCl:urea as plasticizers of high-density polyethylene (HDPE). Despite the improvement of polymer ductility after modiﬁcation with DES, its strength and Tg were not signiﬁcantly changed. For this reason, the authors suggested that the modiﬁcation of DES in the HDPE was as a lubricant rather than a plasticizer, reveling an additional modiﬁer function of DES. More interestingly, the DES modiﬁed-HDPE was blended with starch plasticized with DES. DES-modiﬁcations allowed to blend, for the ﬁrst time, polyoleﬁns (HDPE) to nonchemically modiﬁed carbohydrates (starch) . The thermal and mechanical polymer properties conferred by plasticization with DES can attribute or inﬂuence other properties, speciﬁc of certain applications, as polymer foaming enhancement for the production of 3D porous materials  or water retention capacity, for the production of impermeabilized or hydrophilic materials .
Table 5. Resume of polymer plasticized using deep eutectic solvents and properties acquired by the polymers.
Polymer plasticized DES Properties conferred Ref. ChCl:imidazole 3:7, 2:3 Lower tendency to retrogradation Glycerol:imidazole 1:1, 3:7 Transparent and elastic ﬁlms (thermoplasticized)  Starch Citric acid:imidazole 3:7 Not suitable for starch plasticizing Malic acid:imidazole 3:7 ChCl:urea 1:2 ChCl:imidazole 3:7 Dependent of additive (consult article)  Tailored ductility with DES content ChCl:malic acid 1:1 Lower Tg  Good solubility in water Transparent ﬁlms Lower tensile strength and Young’s modulus ChCl:lactic acid 1:1 (higher ﬂexibility)  Chitosan ﬁlms Higher water vapor permeability (WVP), water solubility, and water sorption Enhanced ﬁlm ﬂexibility ChCl:urea 1:2 Reduced water uptake  Improved ionic conductivity ChCl:malic acid 1:1, ChCl:lactic Transparent ﬁlms acid 1:1, ChCl:citric acid acid 1:1, Elasticity, tensile strength, and WVP tuned by  ChCl:glycerol 1:2 chitosan type and DES composition Chitosan-carboxymethyl Higher thermal stability ChCl:urea 1:2  cellulose membrane Improved ﬂexibility Good mechanical resistance and improved Agar ﬁlms ChCl:urea 1:2  elasticity in comparison to aqueous agar ﬁlms ChCl:glycerol 1:2 ChCl:glucose 1:2 Highly improved ductility ChCl:urea 1:2 Cellulose ﬁlms  Tetrabutylammonium bromide:propylene carbonate 1:2 Improved thermoformability Tetrabutylammonium bromide:ethylene carbonate 1:2 Polymers 2019, 11, 912 14 of 22
Table 5. Cont.
Polymer plasticized DES Properties conferred Ref. Glucose:citric acid 1:1 ChCl:sucrose 1:1, 4:1 Blend of starch and ChCl:citric acid 1:1 Lower Young’s modulus and ductility poly-ε-caprolactone  ChCl:xylose 2:1, 3:1 Enhancement of supercritical foaming (SPCL) Glucose:tartaric acid 1:1 Citric acid:sucrose 1:1 Improved ﬂexibility (higher tensile stress and Young’s modulus) Momordica charantia ChCl:glycerol 1.5:1, 1:1, 1:1.5, Higher thermal stability  bioactive polysaccharide 1:2, 1:3 Higher water adsorption and WVP Antioxidant and antimicrobial activity
5.3. Other Modiﬁcations Some DES can transform a polymer’s structure by disrupting or rearranging its chemical and/or physical networks. Within this context, acidic DES have been used for protein denaturation [107,122]. Tan and the coauthors published the use of urea:guanidine hydrochloride DES as protein denaturant to transform silk ﬁbers into nanoﬁbers . The mentioned study used DES for the combined transformation of two diﬀerent biopolymers, using protein denaturation with DES as a strategy for the modiﬁcation of a more complex biopolymer matrix. Deep eutectic solvents can also be used as reactants for polymer modiﬁcation. An example of this type of modiﬁcation was published by Lian et al., which used zinc chloride:urea 3:10 (molar ratio) DES as both solvent and reactant for lignin modiﬁcation. The zinc contained in DES was partially integrated into the lignin structure by chelation with the lignin functional groups, conferring to the modiﬁed lignin a 4-fold increased molecular weight and enhanced thermal stability . Crosslinking is another possible application of DES as a reactant, as reported by Jordan et al., which used a deep eutectic mixture of hexaketocyclohexane octahydrate:urea to crosslink chitosan .
6. Formulation of DES Materials Using Polymers In the previous sections, DES were explored mainly for polymer processing, as vehicles, additives, modiﬁers, or just as solvents to achieve certain polymeric products or properties. In this section, deep eutectic solvents are the principal agents of the envisioned product, while polymeric systems are used as modiﬁers or carriers. For this purpose, it is important to introduce the concept of therapeutic deep eutectic solvents (THEDES). By deﬁnition, THEDES are deep eutectic solvents for which at least one of the mixture components is an active pharmaceutical ingredient . However, bioactive compounds solubilized in DES are also commonly considered as THEDES . Tuntarawongsa and Phaechamud were the ﬁrst authors to describe the use of polymeric eutectic systems for controlled delivery of active ingredients [127,128]. They used a mixture of two therapeutic compounds—menthol and camphor—to form a therapeutic DES and designed two diﬀerent delivery systems. The addition of eudragit® polymers to the eutectic liquid up to 40% w/w, increased its viscosity, allowing to form a gel product with potential for topic application, using as an advantage the menthol ability to increase skin penetration . Moreover, an injectable formulation was developed. The same DES system incorporating 30% w/w of eudragit® was used for the solubilization and delivery of an additional active ingredient, ibuprofen. The hydrophobic properties of the DES prolonged the time of drug delivery in comparison to a pharmaceutical solvent commonly used for drug solubilization. Additionally, the viscosity enhancement conferred by polymer addition contributed to even higher delivery retardation . The versatility of these polymeric eutectic systems has a high potential to design delivery systems with tailored sustained drug release. A distinct approach was presented by Aroso et al. who developed polymeric delivery systems by impregnating THEDES of menthol:ibuprofen (3:1 molar) in a starch:poly-ε-caprolactone polymer Polymers 2019, 11, 912 15 of 22 blend. The produced 3D structures had higher porous and faster ibuprofen release than the polymeric matrix produced with ibuprofen powder . Furthermore, Mano et al. were the ﬁrst reporting the encapsulation of THEDES in polymeric ﬁbers by electrospinning [9,130]. In 2015, the authors published the encapsulation of ChCl:citric acid (1:1 molar) DES in poly(vinyl alcohol) ﬁbers  and in 2017, the encapsulation of ChCl:mandelic acid (1:2 molar) in gelatin ﬁbers was described . More recently, Liu et al. reported the use of mannose-dimethylurea-water 2:5:5 (molar) as a loading system of lipophilic (curcumin) molecules into a hydrophilic chitosan:alginate hydrogel. The amphiphilic nature of the produced DES could eﬃciently entrap curcumin in its hydrophobic core while being easily incorporated in the hydrogel due to the hydrophilic surrounding. Moreover, the DES external hydrophilic character promoted its spontaneous diﬀusion to the water phase during washing, maintaining the curcumin encapsulated in the hydrogel. The formulation of this system aimed to mimic naturally occurring delivery systems from natural DES (NADES) to biopolymeric matrices, like plants (mimicked by the hydrogel). The authors conﬁrmed similar behavior for DES and Schisandra chinensis fruit extract regarding the transfer of lipophilic molecules to the hydrogel, which supports the prediction that nature has unique delivery systems, by combining NADES and biohydrogels . Despite that the DES have been removed through water washing in their study, it is possible to formulate identical systems without DES elimination from the polymeric matrix, which might be potentially useful for THEDES delivery in aqueous based systems. The last study on polymeric delivery of DES was published by Silva et al., which designed fatty acid antibacterial DES with a tuned melting point for an eﬃcient and stable load into a commercial polymeric gauze and easy diﬀusion from the gauze by melting at physiologic temperature. The tailored DES (lauric acid:myristic acid 1:1 molar) was eﬃciently loaded into the gauze through supercritical dispersion, being highly potential for wound healing applications . Although the delivery of THEDES from polymeric matrices is highly promising, more DES–polymeric products integrating DES as the principal constituent can be developed. A completely diﬀerent system is now presented. Qin et al. developed a DES gel supported with gelatin biopolymer for ionic skin applications. The gel produced from ChCl:ethylene glycol 1:2, with 22% gelatin presented a higher stretchability and toughness than the gels formed from the isolated compounds (ChCl or ethylene glycol), even higher than a conventional hydrogel. The incorporation of pressure and strain sensors into the ﬂexible ionic conductive DES gel allowed accurate monitoring of human ﬁnger bending and multitouch stimuli. Moreover, its nonvolatile character is an advantage over common hydrogels for a long-term duration . This study opens a new platform for the development of nonvolatile sensors based on DES materials.
7. Conclusions Deep eutectic solvents have shown several functionalities and advantages when used in the ﬁeld of polymers. From their properties as green solvent (reusable, nontoxic, etc.), to their use as functional components for polymer synthesis or modiﬁcation, and ﬁnally their use as the main or active component of polymer-based formulations DESs are extremely versatile. The countless possible combinations, ratios, and properties achievable can be tailored to speciﬁc applications. In this review, an overview of the developments involving DES and polymers was presented. Our goal was to inform and inspire the scientiﬁc community to use, adapt and contribute to the available knowledge and to trigger the progress in the ﬁeld.
Author Contributions: Conceptualization, A.R., A.A.M., A.P., and A.R.C.D.; Writing—Original Draft Preparation, A.R. and A.P.; Writing—Review and Editing, A.P., A.A.M., and A.R.C.D.; Supervision, A.A.M. and A.R.C.D.; Project Administration, A.R.C.D.; Funding Acquisition, A.R.C.D. Funding: This work has received funding from the European Union under grant agreement number ERC-2016-CoG-725034 Des.Solve (ERC Consolidator Grant) from Horizon 2020. This work was supported Polymers 2019, 11, 912 16 of 22 by the Associate Laboratory for Green Chemistry- LAQV which is ﬁnanced by national funds from FCT/MCTES (UID/QUI/50006/2019). Conﬂicts of Interest: The authors declare no conﬂicts of interest.
1. Abbott, A.P.; Capper, G.; Davies, D.L.; Rasheed, R.K.; Tambyrajah, V. Novel solvent properties of choline chloride/urea mixtures. Chem. Commun. 2003, 70–71. [CrossRef] 2. Guthrie, F. On eutexia. Proc. Phys. Soc. London 1884, 6, 124–146. [CrossRef] 3. Martins, M.A.R.; Pinho, S.P.; Coutinho, J.A.P. Insights into the Nature of Eutectic and Deep Eutectic Mixtures. J. Solution Chem. 2018.[CrossRef] 4. Zdanowicz, M.; Wilpiszewska, K.; Spychaj, T. Deep eutectic solvents for polysaccharides processing. A review. Carbohydr. Polym. 2018, 200, 361–380. [CrossRef] 5. Francisco, M.; van den Bruinhorst, A.; Zubeir, L.F.; Peters, C.J.; Kroon, M.C. A new low transition temperature
mixture (LTTM) formed by choline chloride+lactic acid: Characterization as solvent for CO2 capture. Fluid Phase Equilib. 2013, 340, 77–84. [CrossRef] 6. Zahn, S.; Kirchner, B.; Mollenhauer, D. Charge Spreading in Deep Eutectic Solvents. ChemPhysChem 2016, 17, 3354–3358. [CrossRef][PubMed] 7. Ashworth, C.R.; Matthews, R.P.; Welton, T.; Hunt, P.A. Doubly ionic hydrogen bond interactions within the choline chloride–urea deep eutectic solvent. Phys.Chem.Chem.Phys. 2016, 18, 18145–18160. [CrossRef] 8. Stefanovic, R.; Ludwig, M.; Webber, G.B.; Atkin, R.; Page, A.J. Nanostructure, hydrogen bonding and rheology in choline chloride deep eutectic solvents as a function of the hydrogen bond donor. Phys. Chem. Chem. Phys. 2017, 19, 3297–3306. [CrossRef] 9. Mano, F.; Aroso, I.M.; Barreiros, S.; Borges, J.P.; Reis, R.L.; Duarte, A.R.C.; Paiva, A. Production of poly(vinyl alcohol) (PVA) ﬁbers with encapsulated natural deep eutectic solvent (NADES) using electrospinning. ACS Sustain. Chem. Eng. 2015, 3, 2504–2509. [CrossRef] 10. Castro, V.I.B.; Mano, F.; Reis, R.L.; Paiva, A.; Duarte, A.R.C. Synthesis and Physical and Thermodynamic Properties of Lactic Acid and Malic Acid-Based Natural Deep Eutectic Solvents. J. Chem. Eng. Data 2018, 63, 2548–2556. [CrossRef] 11. del Monte, F.; Carriazo, D.; Serrano, M.C.; Gutiérrez, M.C.; Ferrer, M.L. Deep eutectic solvents in polymerizations: A greener alternative to conventional syntheses. ChemSusChem 2014, 7, 999–1009. [CrossRef] 12. Anastas, P.T.; Warner, J.C. Green chemistry: theory and practice. Oxford Univ. Press. New York 1998, 30. 13. Choi, Y.H.; van Spronsen, J.; Dai, Y.; Verberne, M.; Hollmann, F.; Arends, I.W.C.E.; Witkamp, G.-J.; Verpoorte, R. Are Natural Deep Eutectic Solvents the Missing Link in Understanding Cellular Metabolism and Physiology? Plant Physiol. 2011, 156, 1701–1705. [CrossRef] 14. Paiva, A.; Craveiro, R.; Aroso, I.; Martins, M.; Reis, R.L.; Duarte, A.R.C. Natural deep eutectic solvents-Solvents for the 21st century. ACS Sustain. Chem. Eng. 2014, 2, 1063–1071. [CrossRef] 15. Vanda, H.; Dai, Y.; Wilson, E.G.; Verpoorte, R.; Choi, Y.H. Green solvents from ionic liquids and deep eutectic solvents to natural deep eutectic solvents. Comptes Rendus Chim. 2018, 21, 628–638. [CrossRef] 16. García-Álvarez, J. Deep Eutectic Mixtures: Promising Sustainable Solvents for Metal-Catalysed and Metal-Mediated Organic Reactions. Eur. J. Inorg. Chem. 2015, 2015, 5147–5157. [CrossRef] 17. Alonso, D.A.; Baeza, A.; Chinchilla, R.; Guillena, G.; Pastor, I.M.; Ramón, D.J. Deep Eutectic Solvents: The Organic Reaction Medium of the Century. European J. Org. Chem. 2016, 2016, 612–632. [CrossRef] 18. Web of Science. Available online: https://apps.webofknowledge.com (accessed on 6 March 2019). 19. Sapir, L.; Stanley, C.B.; Harries, D. Properties of Polyvinylpyrrolidone in a Deep Eutectic Solvent. J. Phys. Chem. A 2016, 120, 3253–3259. [CrossRef] 20. Chen, Z.; Mcdonald, S.; Fitzgerald, P.; Warr, G.G.; Atkin, R. Small angle neutron scattering study of the conformation of poly(ethylene oxide) dissolved in deep eutectic solvents. J. Colloid Interface Sci. 2017, 506, 486–492. [CrossRef] 21. Hammond, O.S.; Bowron, D.T.; Edler, K.J. Liquid structure of the choline chloride-urea deep eutectic solvent (reline) from neutron diﬀraction and atomistic modelling. Green Chem. 2016, 18, 2736–2744. [CrossRef] 22. Stefanovic, R.; Webber, G.B.; Page, A.J. Polymer solvation in choline chloride deep eutectic solvents modulated by the hydrogen bond donor. J. Mol. Liq. 2019, 279, 584–593. [CrossRef] Polymers 2019, 11, 912 17 of 22
23. Hillman, A.R.; Ryder, K.S.; Ismail, H.K.; Unal, A.; Voorhaar, A. Fundamental aspects of electrochemically controlled wetting of nanoscale composite materials. Faraday Discuss. 2017, 199, 75–99. [CrossRef] 24. Freire, M.G.; Cláudio, F.M.; Coutinho, J.A.P.; Marrucho, I.M.; Lopes, J.N.C.; Rebelo, L.P.N. Aqueous biphasic systems: A boost brought about by using ionic liquids. Chem. Soc. Rev. 2012, 41, 4966–4995. [CrossRef] [PubMed] 25. Genies, E.M.; Tsintavis, C. Redox mechanism and electrochemical behayiour of polyaniline deposits. J. Electroanal. Chem. 1985, 195, 109–128. [CrossRef] 26. Dhanalakshmi, K.; Saraswathi, R.; Srinivasan, C. Synthesis and electrochemical stability of polyaniline and polypyrrole in an ambient temperature acetamide-urea-ammonium nitrate eutectic melt. Synth. Met. 1996, 82, 237–243. [CrossRef] 27. Liao, J.; Wu, P.; Bai, Y. Eutectic mixture of choline chloride/urea as a green solvent in synthesis of a coordination polymer: [Zn(O PCH CO )] NH . Inorg. Chem. Commun. 2005, 8, 390–392. [CrossRef] 3 2 2 · 4 28. Monnard, P.A.; Kanavarioti, A.; Deamer, D.W. Eutectic Phase Polymerization of Activated Ribonucleotide Mixtures Yields Quasi-Equimolar Incorporation of Purine and Pyrimidine Nucleobases. J. Am. Chem. Soc. 2003, 125, 13734–13740. [CrossRef] 29. Mota-Morales, J.D.; Gutiérrez, M.C.; Sanchez, I.C.; Luna-Bárcenas, G.; del Monte, F. Frontal polymerizations carried out in deep-eutectic mixtures providing both the monomers and the polymerization medium. Chem. Commun. 2011, 47, 5328–5330. [CrossRef][PubMed] 30. Xu, K.; Wang, Y.; Li, Y.; Lin, Y.; Zhang, H.; Zhou, Y. A novel poly(deep eutectic solvent)-based magnetic silica composite for solid-phase extraction of trypsin. Anal. Chim. Acta 2016, 946, 64–72. [CrossRef][PubMed] 31. Wang, R.; Li, W.; Chen, Z. Solid phase microextraction with poly(deep eutectic solvent) monolithic column online coupled to HPLC for determination of non-steroidal anti-inﬂammatory drugs. Anal. Chim. Acta 2018, 1018, 111–118. [CrossRef] 32. Wang, R.; Mao, Z.; Chen, Z. Monolithic column with polymeric deep eutectic solvent as stationary phase for capillary electrochromatography. J. Chromatogr. A 2018, 1577, 66–71. [CrossRef] 33. Isik, M.; Zulﬁqar, S.; Edhaim, F.; Ruipérez, F.; Rothenberger, A.; Mecerreyes, D. Sustainable Poly(ionic liquid)s
for CO2 Capture based on Deep Eutectic Monomers. ACS Sustain. Chem. Eng. 2016, 4, 7200–7208. [CrossRef] 34. Wei, X.; Wang, Y.; Chen, J.; Xu, P.; Xu, W.; Ni, R.; Meng, J.; Zhou, Y. Poly(deep eutectic solvent)-functionalized magnetic metal-organic framework composites coupled with solid-phase extraction for the selective separation of cationic dyes. Anal. Chim. Acta 2019, 1056, 47–61. [CrossRef] 35. De Leon, A.; Advincula, R.C. Conducting Polymers with Superhydrophobic Eﬀects as Anticorrosion Coating. In Intelligent Coatings for Corrosion Control; Tiwari, A., Rawlins, J., Hihara, L.H., Eds.; Elsevier: Woburn, UK, 2015; pp. 409–430, ISBN 9780124114678. 36. Hillman, A.R.; Ryder, K.S.; Zaleski, C.J.; Fullarton, C.; Smith, E.L. Ion Transfer Mechanisms Accompanying p-doping of Poly(3,4- ethylenedioxythiophene) Films in Deep Eutectic Solvents. Z. Phys. Chem. 2012, 226, 1049–1068. [CrossRef] 37. Prathish, K.P.; Carvalho, R.C.; Brett, C.M.A. Electrochemical characterisation of poly(3,4- ethylenedioxythiophene) ﬁlm modiﬁed glassy carbon electrodes prepared in deep eutectic solvents for simultaneous sensing of biomarkers. Electrochim. Acta 2016, 187, 704–713. [CrossRef] 38. Fernandes, P.M. V.; Campiña, J.M.; Pereira, C.M.; Silva, F. Electrosynthesis of Polyaniline from Choline-Based Deep Eutectic Solvents: Morphology, Stability and Electrochromism. J. Electrochem. Soc. 2012, 159, G97–G105. [CrossRef] 39. Prathish, K.P.; Carvalho, R.C.; Brett, C.M.A. Highly sensitive poly(3,4-ethylenedioxythiophene) modiﬁed electrodes by electropolymerisation in deep eutectic solvents. Electrochem. Commun. 2014, 44, 8–11. [CrossRef] 40. Zou, F.; Huang, X. Electropolymerization in proton-functionalized anilinium salts/glycol deep eutectic solvents. J. Mater. Sci. 2018, 53, 8132–8140. [CrossRef] 41. Hosu, O.; Bârsan, M.M.; Cristea, C.; Săndulescu, R.; Brett, C.M.A. Nanostructured electropolymerized poly(methylene blue) ﬁlms from deep eutectic solvents. Optimization and characterization. Electrochim. Acta 2017, 232, 285–295. [CrossRef] 42. Hosu, O.; Barsan, M.M.; Cristea, C.; Robert, S.; Brett, C.M.A. Nanocomposites based on carbon nanotubes and redox-active polymers synthesized in a deep eutectic solvent as a new electrochemical sensing platform. Microchim. Acta 2017, 184, 3919–3927. [CrossRef] Polymers 2019, 11, 912 18 of 22
43. Bhat, G.; Kandagor, V. Synthetic polymer ﬁbers and their processing requirements. In Advances in Filament Yarn Spinning of Textiles and Polymers; Zhang, D., Ed.; Woodhead Publishing Limited: Cambridge, UK, 2014; pp. 3–30, ISBN 9780857099174. 44. Carriazo, D.; Serrano, M.C.; Gutiérrez, M.C.; Ferrer, M.L.; del Monte, F. Deep-eutectic solvents playing multiple roles in the synthesis of polymers and related materials. Chem. Soc. Rev. 2012, 41, 4996–5014. [CrossRef] 45. Patiño, J.; Gutiérrez, M.C.; Carriazo, D.; Ania, C.O.; Fierro, J.L.G.; Ferrer, M.L.; del Monte, F. DES assisted
synthesis of hierarchical nitrogen-doped carbon molecular sieves for selective CO2 versus N2 adsorption. J. Mater. Chem. A 2014, 2, 8719–8729. [CrossRef] 46. Chen, L.; Deng, J.; Hong, S.; Lian, H. Deep eutectic solvents-assisted cost-eﬀective synthesis of nitrogen-doped hierarchical porous carbon xerogels from phenol-formaldehyde by two-stage polymerization. J. Sol-Gel Sci. Technol. 2018, 86, 795–806. [CrossRef] 47. López-Salas, N.; Carriazo, D.; Gutiérrez, M.C.; Ferrer, M.L.; Ania, C.O.; Rubio, F.; Tamayo, A.; Fierro, J.L.G.; del Monte, F. Tailoring the textural properties of hierarchical porous carbons using deep eutectic solvents. J. Mater. Chem. A 2016, 4, 9146–9159. [CrossRef] 48. Xu, W.; Wang, Y.; Wei, X.; Chen, J.; Xu, P.; Ni, R.; Meng, J. Fabrication of magnetic polymers based on deep eutectic solvent for separation of bovine hemoglobin via molecular imprinting technology. Anal. Chim. Acta 2019, 1048, 1–11. [CrossRef] 49. Viveiros, R.; Rebocho, S.; Casimiro, T. Green Strategies for Molecularly Imprinted Polymer Development. Polymers 2018, 10, 306. [CrossRef] 50. Liang, S.; Yan, H.; Cao, J.; Han, Y.; Shen, S.; Bai, L. Molecularly imprinted phloroglucinol–formaldehyde– melamine resin prepared in a deep eutectic solvent for selective recognition of clorprenaline and bambuterol in urine. Anal. Chim. Acta 2016, 951, 68–77. [CrossRef] 51. Liu, X.-L.; He, W.; Huang, Y.-P.; Yao, H.-F.; Liu, Z.-S.; Chai, M.-H. Green Synthesis of Carbon Nanotubes-Reinforced Molecularly Imprinted Polymer Composites for Drug Delivery of Fenbufen. AAPS PharmSciTech 2018, 19, 3895–3906. [CrossRef] 52. Li, X.; Row, K.H. Puriﬁcation of antibiotics from the millet extract using hybrid molecularly imprinted polymers based on deep eutectic solvents. RSC Adv. 2017, 7, 16997–17004. [CrossRef] 53. Li, G.; Wang, W.; Wang, Q.; Zhu, T. Deep Eutectic Solvents Modiﬁed Molecular Imprinted Polymers for Optimized Puriﬁcation of Chlorogenic Acid from Honeysuckle. J. Chromatogr. Sci. 2016, 54, 271–279. [CrossRef][PubMed] 54. Li, G.; Ahn, W.S.; Row, K.H. Hybrid molecularly imprinted polymers modiﬁed by deep eutectic solvents and ionic liquids with three templates for the rapid simultaneous puriﬁcation of rutin, scoparone, and quercetin from Herba Artemisiae Scopariae. J. Sep. Sci. 2016, 39, 4465–4473. [CrossRef][PubMed] 55. Li, G.; Wang, X.; Row, K.H. Magnetic Solid-phase extraction with Fe3O4/Molecularly Imprinted Polymers Modiﬁed by Deep Eutectic Solvents and Ionic Liquids for the Rapid Puriﬁcation of Alkaloid Isomers (Theobromine and Theophylline) from Green Tea. Molecules 2017, 22, 1061. [CrossRef] 56. Li, G.; Dai, Y.; Wang, X.; Row, K. Molecularly Imprinted Polymers Modiﬁed by Deep Eutectic Solvents and Ionic Liquids with Two Templates for the Simultaneous Solid-Phase Extraction of Fucoidan and Laminarin from Marine Kelp. Anal. Lett. 2018, 2719, 1–15. [CrossRef] 57. Li, G.; Zhu, T.; Row, K.H. Deep eutectic solvents for the puriﬁcation of chloromycetin and thiamphenicol from milk. J. Sep. Sci. 2017, 40, 625–634. [CrossRef][PubMed] 58. Li, X.; Row, K.H. Application of Deep Eutectic Solvents in Hybrid Molecularly Imprinted Polymers and Mesoporous Siliceous Material for Solid-Phase Extraction of Levoﬂoxacin from Green Bean Extract. Anal. Sci. 2017, 33, 611–617. [CrossRef][PubMed] 59. Li, G.; Row, K.H. Magnetic hybrid imprinted polymers with three-templates modiﬁed by DESs for the rapid puriﬁcation of monosaccharide from seaweed. J. Liq. Chromatogr. Relat. Technol. 2017, 40, 1037–1046. [CrossRef] 60. Li, G.; Row, K.H. Magnetic molecularly imprinted polymers for recognition and enrichment of polysaccharides from seaweed. J. Sep. Sci. 2017, 40, 4765–4772. [CrossRef] 61. Li, G.; Wang, X.; Row, K.H. Magnetic molecularly imprinted polymers based on silica modiﬁed by deep eutectic solvents for the rapid simultaneous magnetic-based solid-phase extraction of Salvia miltiorrhiza bunge, Glycine max (Linn.) Merr and green tea. Electrophoresis 2018, 39, 1111–1118. [CrossRef][PubMed] Polymers 2019, 11, 912 19 of 22
62. Tang, W.; Gao, F.; Duan, Y.; Zhu, T.; Ho Row, K. Exploration of deep eutectic solvent-based molecularly imprinted polymers as solid-phase extraction sorbents for screening chloramphenicol in milk. J. Chromatogr. Sci. 2017, 55, 654–661. [CrossRef][PubMed] 63. Meng, J.; Wang, X. Microextraction by Packed Molecularly Imprinted Polymer Combined Ultra-High-Performance Liquid Chromatography for the Determination of Levoﬂoxacin in Human Plasma. J. Chem. 2019, 2019, 1–9. [CrossRef] 64. Liu, Y.; Wang, Y.; Dai, Q.; Zhou, Y. Magnetic deep eutectic solvents molecularly imprinted polymers for the selective recognition and separation of protein. Anal. Chim. Acta 2016, 936, 168–178. [CrossRef] 65. Li, X.; Row, K.H. Application of novel ternary deep eutectic solvents as a functional monomer in molecularly imprinted polymers for puriﬁcation of levoﬂoxacin. J. Chromatogr. B 2017, 1068–1069, 56–63. [CrossRef] 66. Xu, K.; Wang, Y.; Wei, X.; Chen, J.; Xu, P.; Zhou, Y. Preparation of magnetic molecularly imprinted polymers based on a deep eutectic solvent as the functional monomer for speciﬁc recognition of lysozyme. Microchim. Acta 2018, 185.[CrossRef] 67. Li, G.; Row, K.H. Selective extraction of 3,4-dihydroxybenzoic acid in Ilex chinensis Sims by meticulous mini-solid-phase microextraction using ternary deep eutectic solvent-based molecularly imprinted polymers. Anal. Bioanal. Chem. 2018, 410, 7849–7858. [CrossRef] 68. Li, G.; Row, K.H. Ternary deep eutectic solvent magnetic molecularly imprinted polymers for the dispersive magnetic solid-phase microextraction of green tea. J. Sep. Sci. 2018, 41, 3424–3431. [CrossRef] 69. Fu, N.; Li, L.; Liu, X.; Fu, N.; Zhang, C.; Hu, L. Speciﬁc recognition of polyphenols by molecularly imprinted polymers based on a ternary deep eutectic solvent. J. Chromatogr. A 2017, 1530, 23–34. [CrossRef] 70. Ma, W.; Dai, Y.; Row, K.H. Molecular imprinted polymers based on magnetic chitosan with diﬀerent deep eutectic solvent monomers for the selective separation of catechins in black tea. Electrophoresis 2018, 39, 2039–2046. [CrossRef] 71. Zhang, Y.; Cao, H.; Huang, Q.; Liu, X.; Zhang, H. Isolation of transferrin by imprinted nanoparticles with magnetic deep eutectic solvents as monomer. Anal. Bioanal. Chem. 2018, 410, 6237–6245. [CrossRef] 72. Fu, N.; Li, L.; Liu, K.; Kim, C.K.; Li, J.; Zhu, T.; Li, J.; Tang, B. A choline chloride-acrylic acid deep eutectic solvent polymer based on Fe3O4 particles and MoS2 sheets (poly(ChCl-AA DES)@[email protected]) with speciﬁc recognition and good antibacterial properties for β-lactoglobulin in milk. Talanta 2019, 197, 567–577. [CrossRef] 73. Ma, W.; Tang, B.; Row, K.H. Exploration of a ternary deep eutectic solvent of methyltriphenylphosphonium bromide/chalcone/formic acid for the selective recognition of rutin and quercetin in Herba Artemisiae Scopariae. J. Sep. Sci. 2017, 40, 3248–3256. [CrossRef] 74. Mota-Morales, J.D.; Sánchez-Leija, R.J.; Carranza, A.; Pojman, J.A.; del Monte, F.; Luna-Bárcenas, G. Free-radical polymerizations of and in deep eutectic solvents: Green synthesis of functional materials. Prog. Polym. Sci. 2018, 78, 139–153. [CrossRef] 75. Ferreira, V.R.A.; Azenha, M.A.; Pinto, A.C.; Santos, P.R.M.; Pereira, C.M.; Silva, A.F. Development of mesoporous polysaccharide/sol-gel composites with two diﬀerent templating agents: Surfactants and choline chloride-based deep eutectic solvents. Express Polym. Lett. 2019, 13, 261–275. [CrossRef] 76. Maximiano, P.; Mendonça, P. V.; Santos, M.R.E.; Costa, J.R.C.; Guliashvili, T.; Serra, A.C.; Coelho, J.F.J. Eutectic mixtures as a green alternative for eﬃcient catalyst recycling in atom transfer radical polymerizations. J. Polym. Sci. Part A Polym. Chem. 2017, 55, 371–381. [CrossRef] 77. Wang, J.; He, D.; Peng, H.; Khan, M.Y.; Chen, D.; Han, J.; Xie, X.; Xue, Z. Deep eutectic solvents for green and eﬃcient iron-mediated ligand-free atom transfer radical polymerization. Polym. Chem. 2017, 8, 1616–1627. [CrossRef] 78. Mendonça, P. V.; Lima, M.S.; Guliashvili, T.; Serra, A.C.; Coelho, J.F.J. Deep eutectic solvents (DES): Excellent green solvents for rapid SARA ATRP of biorelevant hydrophilic monomers at ambient temperature. Polymer 2017, 132, 114–121. [CrossRef] 79. Li, X.-X.; Zhang, L.-S.; Wang, C.; Huang, Y.-P.; Liu, Z.-S. Green synthesis of monolithic column incorporated with graphene oxide using room temperature ionic liquid and eutectic solvents for capillary electrochromatography. Talanta 2018, 178, 763–771. [CrossRef] 80. Zhou, X.-J.; Zhang, L.-S.; Song, W.-F.; Huang, Y.-P.; Liu, Z.-S. A polymer monolith incorporating stellate mesoporous silica nanospheres for use in capillary electrochromatography and solid phase microextraction of polycyclic aromatic hydrocarbons and organic small molecules. Microchim. Acta 2018, 185, 1–10. [CrossRef] Polymers 2019, 11, 912 20 of 22
81. Park, T.-J.; Lee, S.H. Deep eutectic solvent systems for FeCl3-catalyzed oxidative polymerization of 3-octylthiophene. Green Chem. 2017, 19, 910–913. [CrossRef] 82. Xiong, W.; Wang, Y.; Liu, Q.; Yao, Y.; Xiong, L. Two lanthanide coordination polymers with helical chain structures synthesized ionothermally from a deep-eutectic solvent: Syntheses, structures and luminescence. Inorg. Chem. Commun. 2014, 46, 282–284. [CrossRef] 83. Xiong, W.; Liu, Q.; Liu, C.; Wang, Y. Slow magnetization relaxation in a one-dimensional dysprosium-carboxylate compound based on the linear Dy4 units synthesized ionothermally from a deep-eutectic solvent. Inorg. Chem. Commun. 2014, 48, 18–21. [CrossRef] 84. Meng, Y.; Chen, Y.; Zhang, Z.; Lin, Z.; Tong, M. Gadolinium Oxalate Derivatives with Enhanced Magnetocaloric Eﬀect via Ionothermal Synthesis. Inorg. Chem. 2014, 53, 9052–9057. [CrossRef] 85. Sousa, A.M.M.; Souza, H.K.S.; Latona, N.; Liu, C.; Gonc, M.P. Choline chloride based ionic liquid analogues as tool for the fabrication of agar ﬁlms with improved mechanical properties. Carbohydr. Polym. 2014, 111, 206–214. [CrossRef] 86. Sousa, A.M.M.; Souza, H.K.S.; Uknalis, J.; Liu, S.; Gonc, M.P. Improving agar electrospinnability with choline-based deep eutectic solvents. Int. J. Biol. Macromol. 2015, 80, 139–148. [CrossRef] 87. Orelma, H.; Virtanen, T.; Spoljaric, S.; Lehmonen, J.; Seppa, J.; Rojas, O.J.; Harlin, A. Cyclodextrin-Functionalized Fiber Yarns Spun from Deep Eutectic Cellulose Solutions for Nonspeciﬁc Hormone Capture in Aqueous Matrices. Biomacromolecules 2018, 19, 652–661. [CrossRef] 88. Lin, K.; Ma, R.; Wang, P.; Xin, J.; Zhang, J.; Wolcott, M.P.; Zhang, X. Deep Eutectic Solvent Assisted Facile Synthesis of Lignin-Based Cryogel. Macromolecules 2019, 52, 227–235. [CrossRef] 89. Willberg-Keyriläinen, P.; Hiltunen, J.; Ropponen, J. Production of cellulose carbamate using urea-based deep eutectic solvents. Cellulose 2018, 25, 195–204. [CrossRef] 90. Sánchez-condado, A.; Carriedo, G.A.; Soto, A.P.; Rodríguez-Álvarez, M.J.; García-Álvarez, J.; Hevia, E. Organolithium Initiated Polymerization of Oleﬁns in Deep Eutectic Solvents under Aerobic Conditions. Sustainable Route to Homopolymers, Random Copolymers and Block Copolymers. ChemSusChem 2019. [CrossRef] 91. Loow, Y.L.; New, E.K.; Yang, G.H.; Ang, L.Y.; Foo, L.Y.W.; Wu, T.Y. Potential use of deep eutectic solvents to facilitate lignocellulosic biomass utilization and conversion. Cellulose 2017, 24, 3591–3618. [CrossRef] 92. Tang, X.; Zuo, M.; Li, Z.; Liu, H.; Xiong, C.; Zeng, X.; Sun, Y.; Hu, L.; Liu, S.; Lei, T.; et al. Green Processing of Lignocellulosic Biomass and Its Derivatives in Deep Eutectic Solvents. ChemSusChem 2017, 10, 2695. [CrossRef] 93. Van Osch, D.J.G.P.; Kollau, L.J.B.M.; Van Den Bruinhorst, A.; Asikainen, S.; Rocha, M.A.A.; Kroon, M.C. Ionic liquids and deep eutectic solvents for lignocellulosic biomass fractionation. Phys. Chem. Chem. Phys. 2017, 19, 2636–2665. [CrossRef] 94. Saravana, P.S.; Ho, T.C.; Chae, S.-J.; Cho, Y.-J.; Park, J.-S.; Lee, H.-J.; Chun, B.-S. Deep eutectic solvent-based extraction and fabrication of chitin ﬁlms from crustacean waste. Carbohydr. Polym. 2018, 195, 622–630. [CrossRef] 95. Bai, C.; Wei, Q.; Ren, X. Selective Extraction of Collagen Peptides with High Purity from Cod Skins by Deep Eutectic Solvents. ACS Sustain. Chem. Eng. 2017, 5, 7220–7227. [CrossRef] 96. Mamilla, J.L.K.; Novak, U.; Grilc, M.; Likozar, B. Natural deep eutectic solvents (DES) for fractionation of waste lignocellulosic biomass and its cascade conversion to value-added bio-based chemicals. Biomass Bioenergy 2019, 120, 417–425. [CrossRef] 97. Melro, E.; Alves, L.; Antunes, F.E.; Medronho, B. A brief overview on lignin dissolution. J. Mol. Liq. 2018, 265, 578–584. [CrossRef] 98. Duan, B.; Huang, Y.; Lu, A.; Zhang, L. Recent advances in chitin based materials constructed via physical methods. Prog. Polym. Sci. 2018, 82, 1–33. [CrossRef] 99. Wang, D.; Tang, R. Dissolution of wool in the choline chloride/oxalic acid deep eutectic solvent. Mater. Lett. 2018, 231, 217–220. [CrossRef] 100. Wang, D.; Yang, X.H.; Tang, R.C.; Yao, F. Extraction of Keratin from Rabbit Hair by a Deep Eutectic Solvent and its Characterization. Polymers 2018, 10, 993. [CrossRef] 101. Huang, W.C.; Zhao, D.; Guo, N.; Xue, C.; Mao, X. Green and Facile Production of Chitin from Crustacean Shells Using a Natural Deep Eutectic Solvent. J. Agric. Food Chem. 2018, 66, 11897–11901. [CrossRef] Polymers 2019, 11, 912 21 of 22
102. Esmaeili, M.; Anugwom, I.; Mänttäri, M.; Kallioinen, M. Utilization of DES-Lignin as a Bio-Based Hydrophilicity Promoter in the Fabrication of Antioxidant Polyethersulfone Membranes. Membranes 2018, 8, 80. [CrossRef] 103. Wang, X.; Li, G.; Ho Row, K. Extraction and Determination of Quercetin from Ginkgo biloba by DESs-Based Polymer Monolithic Cartridge. J. Chromatogr. Sci. 2017, 55, 866–871. [CrossRef] 104. Gan, K.; Tang, W.; Zhu, T.; Li, W.; Wang, H.; Liu, X. Enhanced extraction of cleistanthol from Phyllanthus ﬂexuosus by deep eutectic solvent-modiﬁed anion-exchange resin. J. Liq. Chromatogr. Relat. Technol. 2016, 39, 882–888. [CrossRef] 105. Li, X.; Row, K.H. Separation of Polysaccharides by SEC Utilizing Deep Eutectic Solvent Modiﬁed Mesoporous Siliceous Materials. Chromatographia 2017, 80, 1–9. [CrossRef] 106. Bangde, P.S.; Jain, R.D.; Dandekar, P. Alternative approach to synthesize methylated chitosan using deep eutectic solvents, biocatalyst and ‘green’ methylating agents. ACS Sustain. Chem. Eng. 2016, 4, 3552–3557. [CrossRef] 107. Feng, M.; Lu, X.; Zhang, J.; Li, Y.; Shi, C.; Lu, L.; Zhang, S. Direct conversion of shrimp shells to O-acylated chitin with antibacterial and anti-tumor eﬀects by natural deep eutectic solvents. Green Chem. 2019, 21, 87–98. [CrossRef] 108. Abbott, A.P.; Bell, T.J.; Handa, S.; Stoddart, B. Cationic functionalisation of cellulose using a choline based ionic liquid analogue. Green Chem. 2006, 8, 784–786. [CrossRef] 109. Vuoti, S.; Narasimha, K.; Reinikainen, K. Green wastewater treatment ﬂocculants and ﬁxatives prepared from cellulose using high-consistency processing and deep eutectic solvents. J. Water Process Eng. 2018, 26, 83–91. [CrossRef] 110. Wong, C.Y.; Wong, W.Y.; Loh, K.S.; Mohamad, A.B. Study of the plasticising eﬀect on polymer and its development in fuel cell application. Renew. Sustain. Energy Rev. 2017, 79, 794–805. [CrossRef] 111. Sirviö, J.A.; Visanko, M.; Ukkola, J.; Liimatainen, H. Eﬀect of plasticizers on the mechanical and thermomechanical properties of cellulose-based biocomposite ﬁlms. Ind. Crop. Prod. 2018, 122, 513–521. [CrossRef] 112. Wong, W.Y.; Wong, C.Y.; Rashmi, W.; Khalid, M. Choline Chloride:Urea-Based Deep Eutectic Solvent As Additive To Proton Conducting Chitosan Films. J. Eng. Sci. Technol. 2018, 13, 2995–3006. 113. Galvis-Sanchéz, A.C.; Castro, M.C.R.; Biernacki, K.; Gonçalves, M.P.; Biernacki, K.; Souza, H.K.S. Natural deep eutectic solvents as green plasticizers for chitosan thermoplastic production with controlled/desired mechanical and barrier properties. Food Hydrocoll. 2018, 82, 478–489. [CrossRef] 114. Sokolova, M.P.; Smirnov, M.A.; Samarov, A.A.; Bobrova, N. V; Vorobiov, V.K.; Popova, E.N.; Filippova, E.; Geydt, P.; Lahderanta, E.; Toikka, A.M. Plasticizing of chitosan ﬁlms with deep eutectic mixture of malonic acid and choline chloride. Carbohydr. Polym. 2018, 197, 548–557. [CrossRef] 115. Abbott, A.P.; Abolibda, T.Z.; Qu, W.; Wise, W.R.; Wright, L.A. Thermoplastic starch-polyethylene blends homogenised using deep eutectic solvents. RSC Adv. 2017, 7, 7268–7273. [CrossRef] 116. Martins, M.; Aroso, I.M.; Reis, R.L.; Duarte, A.R.C.; Craveiro, R.; Paiva, A. Enhanced performance of supercritical ﬂuid foaming of natural-based polymers by deep eutectic solvents. AIChE J. 2014, 60, 3701–3706. [CrossRef] 117. Shaﬁe, H.M.; Samsudin, D.; Yusof, R.; Gan, C.-Y. Characterization of bio-based plastic made from a mixture of Momordica charantia bioactive polysaccharide and choline chloride/glycerol based deep eutectic solvent. Int. J. Biol. Macromol. 2018, 118, 1183–1192. [CrossRef] 118. Zdanowicz, M.; Spychaj, T.; Honorata, M. Imidazole-based deep eutectic solvents for starch dissolution and plasticization. Carbohydr. Polym. 2016, 140, 416–423. [CrossRef] 119. Adamus, J.; Spychaj, T.; Zdanowicz, M.; J˛edrzejewski,R.; Roman, J. Thermoplastic starch with deep eutectic solvents and montmorillonite as a base for composite materials. Ind. Crop. Prod. 2018, 123, 278–284. [CrossRef] 120. Almeida, M.R.; Magalh, J.M.C.S.; Química, D.D.E.; Engenharia, F. De; Porto, U.; Frias, R.R. The role of choline chloride-based deep eutectic solvent and curcumin on chitosan ﬁ lms properties. Food Hydrocoll. 2018, 81, 456–466. [CrossRef] 121. Wong, C.Y.; Wong, W.Y.; Walvekar, R.; Loh, K.S.; Khalid, M.; Lim, K.L. Eﬀect of deep eutectic solvent in proton conduction and thermal behaviour of chitosan-based membrane. J. Mol. Liq. 2018, 269, 675–683. [CrossRef] Polymers 2019, 11, 912 22 of 22
122. Tan, X.; Zhao, W.; Mu, T. Controllable exfoliation of natural silk ﬁbers into nanoﬁbrils by protein denaturant deep eutectic solvent: Nanoﬁbrous strategy for multifunctional membranes. Green Chem. 2018, 20, 3625–3633. [CrossRef] 123. Lian, H.; Hong, S.; Carranza, A.; Mota-Morales, J.D.; Pojman, J.A. Processing of lignin in urea–zinc chloride deep-eutectic solvent and its use as a ﬁller in a phenol-formaldehyde resin. RSC Adv. 2015, 5, 28778–28785. [CrossRef] 124. Jordan, T.; Yu, Z.L.; Yu, S.H.; Antonietti, M.; Fechler, N. Porous nitrogen-doped carbon monoliths derived from biopolymer-structured liquid precursors. Microporous Mesoporous Mater. 2018, 255, 53–60. [CrossRef] 125. Duarte, A.R.C.; Ferreira, A.S.D.; Barreiros, S.; Cabrita, E.; Reis, R.L.; Paiva, A. A comparison between pure active pharmaceutical ingredients and therapeutic deep eutectic solvents: Solubility and permeability studies. Eur. J. Pharm. Biopharm. 2017, 114, 296–304. [CrossRef] 126. Santos, F.; PS Leitão, M.; C Duarte, A. Properties of Therapeutic Deep Eutectic Solvents of L-Arginine and Ethambutol for Tuberculosis Treatment. Molecules 2018, 24, 55. [CrossRef] 127. Tuntarawongsa, S.; Phaechamud, T. Polymeric Eutectic System. Adv. Mater. Res. 2012, 528, 180–183. [CrossRef] 128. Tuntarawongsa, S.; Phaechamud, T. Polymeric Eutectic Drug Delivery System. J. Met. Mater. Miner. 2012, 22, 27–32. 129. Aroso, I.M.; Craveiro, R.; Rocha, Â.; Dionísio, M.; Barreiros, S.; Reis, R.L.; Paiva, A.; Duarte, A.R.C. Design of controlled release systems for THEDES—Therapeutic deep eutectic solvents, using supercritical ﬂuid technology. Int. J. Pharm. 2015, 492, 73–79. [CrossRef] 130. Mano, F.; Martins, M.; Sá-nogueira, I.; Barreiros, S.; Borges, J.P.; Reis, R.L.; Duarte, A.R.C.; Paiva, A. Production of Electrospun Fast-Dissolving Drug Delivery Systems with Therapeutic Eutectic Systems Encapsulated in Gelatin. AAPS PharmSciTech 2017, 18, 2579–2585. [CrossRef][PubMed] 131. Liu, Y.; Zhang, Y.; Chen, S.N.; Friesen, J.B.; Nikoli´c,D.; Choules, M.P.; McAlpine, J.B.; Lankin, D.C.; Gemeinhart, R.A.; Pauli, G.F. The inﬂuence of natural deep eutectic solvents on bioactive natural products: Studying interactions between a hydrogel model and Schisandra chinensis metabolites. Fitoterapia 2018, 127, 212–219. [CrossRef] 132. Silva, J.M.; Akkache, S.; Araújo, A.C.; Masmoudi, Y.; Reis, R.L.; Badens, E.; Duarte, A.R.C. Development of innovative medical devices by dispersing fatty acid eutectic blend on gauzes using supercritical particle generation processes. Mater. Sci. Eng. C 2019, 99, 599–610. [CrossRef] 133. Qin, H.; Owyeung, R.E.; Sonkusale, S.R.; Panzer, M.J. Highly stretchable and nonvolatile gelatin-supported deep eutectic solvent gel electrolyte-based ionic skins for strain and pressure sensing. J. Mater. Chem. C 2019, 7, 601–608. [CrossRef]
© 2019 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).